Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

PAPER

Cite this: Phys. Chem. Chem. Phys., 2015, 17, 9812

View Journal | View Issue

Probing the morphological influence on solid electrolyte interphase and impedance response in intercalation electrodes Chien-Fan Chen and Partha P. Mukherjee* Solid electrolyte interphase (SEI) formation, due to the electrochemical reaction between the salt and solvent in the electrolyte, is a key contributor to the electrode performance decay in lithium-ion batteries. The active particle morphology and electrode microstructure aﬀect the side reaction rate and hence the SEI induced interfacial transport and impedance behavior. The change resistance due to the variation of SEI thickness can be inferred from electrochemical impedance spectroscopy. In this study, we proposed a microstructure-aware impedance model to predict the eﬀect of electrode microstructure on

Received 9th December 2014, Accepted 9th March 2015

impedance response. Our model successfully captures the influence of active particle morphology on the SEI

DOI: 10.1039/c4cp05758a

and compositional variations have been considered. The critical influence of active material morphology,

formation and corresponding impedance characteristics. Diﬀerent electrode realizations with microstructural mean particle size, binder and electrolyte volume fractions on the SEI formation and impedance behavior

www.rsc.org/pccp

reveals the underlying interdependences of the interfacial and transport resistance modes.

Introduction Lithium-ion batteries (LIBs), due to their favorable energy density and power capability, are considered as the candidate of choice for vehicle electrification.1–4 Significant efforts are focusing on predicting and extending the life, performance and safety of LIBs to satisfy the increasing demand of LIBs. Mechanical and chemical degradation modes, such as fracture in the electrode active particles due to diffusion induced stress5–8 and the solid electrolyte interphase (SEI) formation,9,10 pose a significant bearing on the LIB life and performance decay in terms of capacity fade and impedance rise.11,12 The SEI is a thin layer (5–300 nm)13 which forms at the interface between the active material and electrolyte, especially on the negative electrode (anode), during the charging process of LIBs.14 Although the SEI formation protects battery components (electrode and electrolyte) from undesired reduction and oxidation,15,16 it also comes with several disadvantages. The SEI formation consumes the active lithium ions and solvent,17,18 and leads to capacity fade. In addition, the thin layer also hinders the intercalations of lithium ion between the electrolyte and the active material, and increases the cell resistance.19–22 The SEI layer thickness varies with the operation condition (temperature and charge rate) and the morphology (i.e. size and shape) of the active material particles in the anode.23–26 Department of Mechanical Engineering, Texas A&M University, College Station, TX, USA. E-mail: [email protected]

9812 | Phys. Chem. Chem. Phys., 2015, 17, 9812--9827

Therefore, particle size distribution and morphology of the active material inside the electrode microstructure become an important factor to control the chemical degradation level under the same operation condition. Electrochemical impedance spectroscopy (EIS) is a powerful technique to analyze the response of an electrochemical system, which is subjected to a small perturbation of voltage or current.27–29 The cell resistances (i.e. charge transfer resistance, solid-phase diffusion resistance and SEI resistance) can be quantified and studied via the impedance response.28,30–37 From previous studies, the microstructure has been proven to have influence to the charge transfer resistance and diffusion resistance.38,39 In the context of impedance modeling, the mathematical EIS model for active particles was originally proposed by Tribollet et al.40,41 Based on the active particle impedance model, the EIS response of porous electrodes was further developed by Meyers et al. and Huang et al.28,42 The porous electrode EIS model combines the porous electrode theory43–45 with the phenomenological approach of active particles to describe the impedance of a homogeneous electrode. Previous numerical EIS simulation for SEI studies which based on the porous electrode theory (developed by Meyers et al.28 and Huang et al.42) did not consider the fact that the SEI thickness varies with the morphology of carbon active materials. Since the side reaction rate and time vary with the morphology of active material,46 the SEI thickness inside the electrode is not uniform and hence the impedance response. To include the morphological eﬀect, we proposed a microstructureaware impedance model to improve the impedance prediction.

This journal is © the Owner Societies 2015

View Article Online

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

Paper

PCCP

In this model, the electrochemical properties of each active particle in the electrode, such as SEI thickness, were evaluated during the charging process. Subsequently, according to the evaluated electrochemical properties, the corresponding impedance response for the electrode microstructure can be predicted. In this study, the canonical mode of chemical degradation (i.e. SEI formation) and concomitant impedance response are studied for diﬀerent electrode microstructural and compositional variations. In particular, the influence of active particle morphology, size distribution, binder, and electrolyte volume fractions is investigated. The microstructure-aware computational model predictions are envisioned to provide fundamental insight into the influence of electrode microstructures on the chemical degradation mode and virtual diagnosis of impedance response.

Microstructure-aware impedance model As mentioned, in order to include the morphological eﬀect of active material to the impedance response, the electrochemical properties of each active particle should be evaluated accordingly. The schematic diagram of our microstructure-aware impedance model is as shown in Fig. 1. First, microstructures with diﬀerent particle-size distribution and composition was constructed, which aﬀect the active interfacial area and porosity. The primary components in the generated microstructures are the active material, electrolyte, and binder. The active materials are generated using the sequential generation method of piling in the active material particles and then randomly distributing the particles within the void space. All particles are prohibited from overlapping in the domain. The binder was added to a structure in the shape of a concave meniscus in locations where material surfaces got close together. The amount of binder utilized was varied by volume fraction. Based on the assigned active particle morphology in the microstructure, the lithiation– delithiation and side reaction (SEI formation) of active particles were simulated during cycling accordingly. With the evaluated electrochemical properties, such as SEI thickness and state of

Fig. 1

charge (SOC), the corresponding impedance response can be evaluated from the analytical solution of EIS of porous electrode.28 It is important to note that, in this study, the active particles are considered to homogeneously disperse throughout the electrode microstructure. The aggregation of active material and hence the effect on the structure of SEI film47 is not taken into account. The active particle aggregation will be included in the future development of this impedance model. Impedance response of a porous microstructure The analytical solution of microstructure-aware impedance model was based on the model developed by Meyers et al.28 The values used in the calculation of impedance and the meaning of parameters in the equations are presented in Table 1. The schematic diagram of diﬀerent active material morphologies is shown in Fig. 2(a). The aspect ratio a and b are set to make the side surface area much smaller than the reactive surface area (10 times smaller). In Fig. 2(b) and (c), an equivalent circuit of the interface and a sample of the impedance response are displayed. The first semicircle of the high frequency accounts for the SEI resistance and the second semicircle of the middle frequency accounts for the charge transfer resistance. Larger diameter of semicircle corresponds to larger resistance. The slope of the impedance tail corresponds to the solid-phase diﬀusion resistance. Higher slope of this tail corresponds to smaller diﬀusion resistance and lower values of the slope signify enhanced solid phase diﬀusion resistance. In this study, we considered an electrode-only model, specifically for a representative anode active particle. Therefore, all the parameters in the following EIS model refer to a typical graphite active material. It is important to note that since graphite is chosen as the representative active material, the eﬀect of active particle volume change on the SEI formation and corresponding impedance response is neglected in this study. This important eﬀect of volume change is left as a future exercise. From the equivalent circuit (Fig. 2(b)), the impedance Z of active particles can be expressed as follows. The admittance Y for active particle can be expressed as eqn (1).where Rct,1 and

Schematic diagram of the microstructure-aware impedance model, which considers the morphological eﬀect of active material.

This journal is © the Owner Societies 2015

Phys. Chem. Chem. Phys., 2015, 17, 9812--9827 | 9813

View Article Online

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

PCCP

Paper

Fig. 2 (a) The morphology of spherical, cylinder and platelet active materials. Cylinder particles: a = 5. Platelet particles: a = 10 and b = 10. (b) Equivalentcircuit diagram. (c) Sample of electrochemical impedance spectroscopy. The first semicircle on the left accounts for the SEI resistance. The second semicircle accounts for the charge transfer resistance. The slope of the impedance tail account for the solid-phase diﬀusivity.

Y¼

1 ¼ Z

1 Rpart Rct;1 þ Ys 1 þ joCdl;1

Rpart Rct;1 þ Ys

þ Rfilm þ

Rct;2 1 þ joRct;2 Cdl;2

þ joCfilm

(1)

Rpart/Ys are the charge transfer and diﬀusion resistance between the solid phase and SEI layer which can be calculated from eqn (2) and (3) when particle radius r = Rs. The SEI resistance Rfilm and capacitance Cfilm can be calculated from Table 2. Rct;1 ¼

RT I0 ðrÞðaa þ ac ÞF

Rpart ¼

@U Rs @cs FDs

(2)

(3)

with the slope of open circuit potential (qU/qcs) can be expressed as eqn (4);48 the exchange current density Ii,0 is a function of state of charge xi,surf as eqn (5). The state of charge xi,surf is defined as the ratio between surface concentration and the maximum surface concentration csurf/cmax @U 0:63562 0:37 ¼ h 2 i h 2 i @cs 22:523xi;surf 3:653 þ1 28:348xi;surf 13:44 þ1 49:9789eð49:9789xi;surf 43:3789Þ

(4)

33:9111e49:2036xi;surf 106:6e254:4xi;surf Ii,0 = ki(ci,max xi,surfci,max)0.5(xi,surfci,max)0.5c0.5 e

9814 | Phys. Chem. Chem. Phys., 2015, 17, 9812--9827

(5)

The value of Ys for the diﬀusion resistance in eqn (1) can be calculated from eqn (6)–(8) for spherical, cylinder and platelet particles. rﬃﬃﬃﬃﬃﬃ rﬃﬃﬃﬃﬃﬃ jw jw tanh Rs Rs Ds Ds Ys ¼ for sphere (6) rﬃﬃﬃﬃﬃﬃ jw tanh Rs Ds Rs Ys ¼

rﬃﬃﬃﬃﬃﬃ rﬃﬃﬃﬃﬃﬃ jw jw I1 R s Ds Ds for cylinder rﬃﬃﬃﬃﬃﬃ jw I0 R s Ds

rﬃﬃﬃﬃﬃﬃ rﬃﬃﬃﬃﬃﬃ jw jw Ys ¼ Rs tanh Rs for platelet Ds Ds

(7)

(8)

According to the previous study, Rct,1 is the major factor, which determines the charge transfer resistance (diameter of right semicircle in Fig. 2(c)) and is dominated by the exchange current density I0 and temperature T. The change in the slope of the low frequency tail (solid-phase diﬀusion resistance) is due to the variation of diﬀusivity Ds and qU/qcs. The SEI resistance (diameter of left semi-circle in Fig. 2(c)) is only aﬀected by the SEI thickness as shown in Table 2.28,42 By implementing the admittance Y calculated from eqn (1), we can evaluate the EIS for the porous microstructure. The impedance Z for the porous microstructure can be expressed as eqn (9). s k 2 3 þ cosh u 2þ L 4 k s 5 (9) 1þ Z¼ u sinh u kþs

This journal is © the Owner Societies 2015

View Article Online

Paper Table 1

PCCP Parameters and values

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

Parameters (i = p, n) a ce ci,max Cfilm Ds F Ii,0 Iapp i0f Ji Js kp kn kf L Mf Ncycle Qp Qs R Rct,1 Rct,2 Cdl,1 Cdl,2 Rfilm Rs Si T Ui Uref,f xi,avg xi,surf Y Z aa,i ac,i ac,f eSEI dSEI Zi Zs s k rf rSEI fi

Table 2

Specific surface area (cm ) Electrolyte concentration (mol cm3) Maximum Li+ concentration in the solid phase (mol cm3) SEI capacitance (F cm2) Solid phase diﬀusion coeﬃcient for Li+ for each electrode (cm2 s1) Faraday’s constant Exchange current density for each electrode Applied current (A) Exchange current density for the formation of film (A cm2) Current density for each electrode (A cm2) Side reaction current (A cm2) Rate constant for cathode (A cm2.5 mol1.5) Rate constant for anode (A cm2.5 mol1.5) Rate constant for SEI formation (A cm2.5 mol1.5) Length of electrode (cm) Molecular weight of SEI (g mol1) Total number of cycles Charge capacity (A h) Capacity loss (A h) Gas constant Charge transfer resistance between solid phase and SEI (O cm2) Charge transfer resistance between SEI and electrolyte (O cm2) Capacitance of the double layer between solid phase and SEI (F cm2) Capacitance pf the double layer between SEI and electrolyte (F cm2) SEI resistance (O cm2) Active material particle radius in electrode Eﬀective electroactive surface area for each electrode (cm2) Temperature (K) Open circuit potential of each electrode (V) Open circuit potential for SEI (V) Ratio of average Li+ concentration to the maximum Li+ concentration for each electrode Ratio of surface Li+ concentration to the maximum Li+ concentration for each electrode Admittance for the single particle (O1 cm2) Impedance for the porous electrode (O cm2) Anodic transfer coeﬃcient Cathodic transfer coeﬃcient Cathodic transfer coeﬃcient for the SEI formation SEI permittivity SEI thickness (cm) Overpotentials for the Li+ intercalation for each electrode (V) Side reaction overpotential (V) Electrical conductivity of solid phase (S cm1) Ion conductivity of electrolyte (S cm1) SEI density (g cm3) SEI resistivity (O m) Potential for each electrode

SEI capacitance and resistance

Morphology Spherical Cylinder Platelet

Value 1

The SEI capacity Cfilm (F cm2)

The SEI resistance Rfilm (O cm2)

eSEI ðRs þ dSEI Þ dSEI Rs eSEI 1 Rs lnððRs þ dSEI Þ=Rs Þ eSEI dSEI

rSEI dSEI Rs Rs þ dSEI rSEIRsln((Rs + dSEI)/Rs) rSEIdSEI

where L ¼ u

ks kþs

1=2

aY

1=2

(10)

The average of single particle admittance aY is calculated from averaging the admittance with the surface area as

This journal is © the Owner Societies 2015

Ð1 8 aY ¼ 4p 0 NðrÞYðrÞr2 dr for sphere > > > < Ð1 aY ¼ 2pa 0 NðrÞYðrÞr2 dr for cylinder > > > Ð1 : aY ¼ ab 0 NðrÞYðrÞr2 dr for platelet

1 103 3.055 102 1 109 96 487 0.7

0.2252 0.4854 1.6 1013 0.005 74

8.3143 0 1 105 0 4 104 298 0.4

0.5 0.5 0.5 8.854 1013

2.4 103 1.1 103 2.1 5 107

(11)

where N(r) is the number density of particle radius r. In this work, we use the modified logarithm Gaussian distribution proposed by Meyers et al.28 as eqn (12). The benefit of using eqn (12) is that controlling the electrode design parameters (specific area a, volume fraction es and mean particle radius) is straight forward. 2 0 12 3 rala 2 j2 3 ln 7 6 B 1 ðala Þ3 e 4 3es le C 6 C 7 NðrÞ ¼ 4 7 pﬃﬃﬃ 5 exp6B @ A 2 5 4 j r ð4pÞ9ðes le Þ pj (12)

5 rala exp ln 3es le 2

Phys. Chem. Chem. Phys., 2015, 17, 9812--9827 | 9815

View Article Online

PCCP

Paper

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

Here, j the sharpness of distribution function can be used to decide the mean particle radius. la and le are the adjusted constants for the morphology, which can be defined as 8 8 1 for sphere 1 for sphere > > > > > > > > > > > > > > > > > > > 2p > > 2p > > : : for platelet for platelet ab 3ab From eqn (12) and (13), we can make sure the specific area and the volume fraction of active material maintain constant when changing particle morphology ð1 ð1 AðrÞNðrÞdr and es ¼ VðrÞNðrÞdr (14) a¼ 0

0

Here A(r) and V(r) are the surface area and volume of active material with particle radius r. One should notice that the microstructure constructed in Fig. 1 is according to the particle size distribution defined from eqn (12). Delithiation–lithiation and side reaction of active materials The evaluation of particle electrochemical properties and SEI formation during delithiation–lithiation were based on the method developed by Rahimian et al.24,46 This method simulated the evolution of lithiation concentration inside the active particles and the side reaction under a certain flux of lithiation and delithiation.49,50 The mathematical formulation is briefly expressed as follows. By applying the average volume technique, Fick’s second law can be simplified as eqn (15)–(20) to predict the diffusion of lithium ion in the cathode (p) and anode (n).24 dxi;ave 3Ji ¼ dt FRs ci;max dxi;ave 2Ji ¼ dt FRs ci;max dxi;ave Ji ¼ dt FRs ci;max xi;surf xi;ave ¼

xi;surf xi;ave ¼

for sphere

for cylinder

Rs Ji 4FDs;i ci;max

(16)

ci;ave ci;surf and xi;surf ¼ ci;max ci;max

In the present paper, xi,surf also can be referred to the state of charge (SOC) of particles. Js in eqn (21) is the side reaction current density which can be calculated from Tafel kinetics as eqn (23). 8 9 ac;f F > < Js ¼ i0f exp = Zs ; Charge > RT (23) > > : ; Js ¼ 0; Discharge Zs ¼ fn Uref

xi;surf xi;ave

(24)

i0,f = kf ceF

(25)

The formation of SEI thickness dSEI can be evaluated from the side reaction current as shown in eqn (26). ddSEI Js Mf ¼ dt rf F

(26)

The Butler–Volmer equation was used to update the reaction current density Ji after each time step. The Butler–Volmer equation can be expressed as eqn (27).

aa;i F ac;i F Ji ¼ Ii;0 exp Zi exp Zi (27) RT RT Ii,0 is the exchange current density which is a function of SOC xi,surf as shown in eqn (5). The over-potentials Zi for the interaction reaction for anode and cathode can be calculated from eqn (28) and (29). Zp = fp UP

Iapp charge Zn ¼ fn Un Rfilm þdischarge Sn

(28) (29)

for sphere

(18)

for cylinder

(19)

with N the number of steps; yi the loss of SOC which can be calculated from eqn (31)–(33).

(17)

for platelet

(20)

Here i denotes either anode (n) or cathode (p). The reaction current density Jp and Jn, side reaction current density Js, and the applied current Iapp follow the charge conservation (eqn (21)). xi,ave and xi,surf are defined in eqn (22). Jp ¼

Iapp Rfilm Sn

where Rfilm is the SEI resistance and can be calculated from Table 2 for different morphologies of particles. The exchange current density for the side reaction i0,f is calculated from eqn (25).

yi ¼ Rs Ji ¼ 3FDs;i ci;max

(22)

The loss of capacity are represented from the loss or gain of SOC xi,surf, and xi,surf was updated after each charging process from eqn (30) þcathode xi;N;surf ¼ xi;N1;surf yi;N1 (30) anode

for platelet

Rs Ji 5FDs;i ci;max

(15)

xi;ave ¼

Iapp Iapp and Jn ¼ Js Sp Sn

9816 | Phys. Chem. Chem. Phys., 2015, 17, 9812--9827

(21)

Qs ¼

Qs Qmax

ð t¼charge time

(31)

ðJs Sn Þdt

(32)

Iapp Sn dt

(33)

0

Qmax ¼

ð t¼charge time 0

In the active particle, the SOC (xi,surf) during discharge–charge can be obtained from eqn (15)–(20). The SOC dominates the

This journal is © the Owner Societies 2015

View Article Online

Paper

PCCP

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

Results and discussion

Fig. 3 The comparison between the experimental EIS and the simulated EIS from our model after the 10th charge–discharge cycle (C/10 rate). Experimental data is adapted from ref. 35.

value of qU/qcs slope and exchange current density I0 in the impedance model as shown in eqn (4) and (5), respectively. The most important part in the present model is calculating the growing of SEI thin layer as shown in eqn (26). The thickness of the SEI thin layer generates additional resistance (Table 2 and eqn (1)) and affects the impedance response. Since the diﬀusion distance and specific capacity (mA h g1) varies with the active particle radius and morphology, the SOC and charging time of active particles inside an electrode is diﬀerent. The SOC of particles aﬀects the anode potential fn which has influence on the side reaction rate as shown in eqn (24). The charging time also determined the SEI thickness as eqn (26). Due to the variation of side reaction rate and charging time of active particles, the electrodes with diﬀerent particle radius distribution should have diﬀerent impedance response. By investigating the impedance response from different design of electrodes, we can (1) find an eﬀective method to design an electrode which has less SEI resistance (2) study the trade-oﬀ between the SEI resistance, charge transfer resistance and solid-phase diﬀusion resistance. It is important to note the eﬀect of phase transformation, such as in LiFePO4, and relevant dependence of solid-state transport on exposed surface facets and crystallographic orientation on the formation of SEI and the charge transfer characteristics are not included in the current version of the microstructure-aware impedance model. These important aspects will be discussed in a future study. The comparison between our model and the experimental EIS is as shown in Fig. 3.35 The trend of simulated EIS shows good agreement with the experimental EIS. The error is mainly due to the selection of particle-size distribution. The comparison shows the ability of our model to study the degradation of anodes.

This journal is © the Owner Societies 2015

In order to study the SEI formation and the corresponding impedance response of the LIB anode, we used the microstructure-aware impedance model as mentioned in previous section. The impedance study includes three stages. First, we calculated the SEI thickness dSEI and the SOC xi,surf for active particles with diﬀerent particle-size distribution (0.3–20 mm) and morphology (spherical, cylindrical and platelet particles) inside the electrode microstructure during the charging– discharging process. The particle-size distribution (0.3–20 mm) selected in this study is based on the thickness of SEI film. Since the SOC of small particles reaches its maximum value faster than large particle under the same lithiation rate, therefore, the SEI thickness is significantly small for smaller particle size, e.g. below 0.3 mm. The importance of nanoscale size effect, e.g. in the range of 0.1–0.01 mm, and corresponding influence on crystallographic orientation, columnar ordering and solidphase transport have been shown in our recent work.51 The specific influence of such morphological aspects on the SEI formation and impedance response will be considered in a future study. Second, the corresponding lithium concentration (e.g. SOC) and SEI thickness is used to calculate the admittance Y of active particle from eqn (1). Third, the admittance for active particles was integrated with the particle radius r as eqn (11) to get the impedance response for porous microstructure electrode with different electrode designs. In this section, we study the porous electrode designed with diﬀerent specific area (cm1), mean particle radius of active material, morphology of active material, and diﬀerent volume fraction of binder. The parameters used in the simulations are given in Table 1 according to previous researches for solid-phase diﬀusion, side reaction, and porous electrode EIS simulations.24,28,42 One should notice that the influence of microstructure to the electrical and ionic conductivity was not considered in this study. Eﬀect of active material morphological on SEI formation and impedance response During lithiation and delithiation process, all active materials were performed with the same current density Ji. The charge and discharge rates were set to 0.5 C (828 mA). The simulation for diﬀerent microstructure designs were operated with 2000 cycles. The SEI thickness dSEI, exchange current density I0, and qU/qcs was recorded after the end of charging process of each cycle. At the end of the charge process of each cycle (charging time = 3600 s), the EIS was calculated to observe the SEI resistance and the degradation of anodes. The active particles with diﬀerent size and morphology were systematically studied in this section. The results show in the following section can help us to understand the impedance response for diﬀerent electrode microstructures in the later sections. Influence of spherical particle radius. Since the particle size varies in the electrode, the impedance for the active materials with diﬀerent particle radius has been studied. The impedance response for active materials, which calculated from eqn (1),

Phys. Chem. Chem. Phys., 2015, 17, 9812--9827 | 9817

View Article Online

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

PCCP

Paper

Fig. 4 (a) The SEI thickness, (b) SOC, (c) qU/qcs and (d) exchange current density of spherical particles with the radius of 0.5, 1, 2, 5 and 10 mm during the first 2000 discharge–charge cycles.

will later be used to calculate the impedance response for the porous electrode. The SEI thicknesses calculated after the end of charging process of each cycle for diﬀerent particle radius are shown in Fig. 4(a). The SEI thickness decreases as particle radius increases when the radius is larger than 1 mm. This result can be explained by the relation between SOC and side reaction rate. Since the SOC increases slower in larger particles, as

shown in Fig. 4(b), the potentials of larger particles increase less than smaller particles after the same charge duration. Due to the low potential variation, larger particles have less side reaction current as shown in eqn (23) and (24). On the opposite, when the radius is smaller than 1 mm, the SEI thickness decreases as the particle radius decreases. The small particles have opposite results because the SOC of small particles increases very fast, which causes the particles to reach their

Fig. 5 (a) Impedance response of a representative spherical active particle after 500, 1000 and 2000 discharge–charge cycles with 2 mm radius spherical active particles. (b) Impedance response of representative spherical active particles after 500 discharge–charge cycles with radius 2, 5 and 10 mm radius spherical active particles.

9818 | Phys. Chem. Chem. Phys., 2015, 17, 9812--9827

This journal is © the Owner Societies 2015

View Article Online

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

Paper

maximum SOC and stop the electrochemical reaction before the end of charge time (3600 s). Therefore, the submicrometer particles have short side reaction time and thin SEI thickness. The SOC, exchange current I0 and qU/qcs, with diﬀerent particle radius after diﬀerent cycles, are shown in Fig. 4(b)–(d) respectively. The value of exchange current I0 and qU/qcs are dominated by the SOC of particle. According to eqn (15), larger particles have lower SOC after the same charge time. Additionally, the SOC decreases during cycling due to the capacity lost from the side reaction as shown in Fig. 4(b). Therefore, as shown in Fig. 4(c), the slope qU/qcs decreases as the number of cycles and particle size increase. For the exchange current density, since the formulation of exchange current density I0 is a second order equation which has the maximum value when SOC = 0.5, the exchange current density increases (decreases) with the increase of SOC when SOC o 0.5 (SOC 4 0.5). Hence, the exchange current density of particles radius of 0.5 and 1 mm increase during cycling, and 2 mm particles have the largest exchange current density after 3600 s of charge time as shown in Fig. 4(d). From the result of SEI thickness, exchange current density I0, and qU/qcs, the impedance response for active particles with diﬀerent radius can be evaluated. Fig. 5(a) shows the impedance response of 1 mm active particles after 500, 1000 and 2000 cycles. The SEI resistance (first semicircle on the left)

PCCP

increases with cycling. The increase of SEI resistance is due to the growth of SEI thickness during cycling as shown in Fig. 4(a). Fig. 5(b) shows that the impedance response varies with particle radius because of the diﬀerence in SEI thickness and SOC. As shown in the result, 10 mm particle has the smallest SEI resistance since it has the thinnest SEI thickness (Fig. 4(a)). However, 10 mm particle has the largest charge transfer resistance because it has the lowest exchange current density I0 as shown in Fig. 4(d). In addition, 10 mm particle also has the largest solid-phase diﬀusion resistance, which is because (1) the radius of particles increases the diﬀusion distance of lithium ion (2) larger particles has smaller value of qU/qcs as shown in Fig. 4(c). One should notice that the SEI resistance and the charge transfer resistance have no eﬀects on the diﬀusion resistance because of the accepted nature of SEI and charge transfer resistance.42 Influence of particle morphology. The morphological eﬀects was performed with spherical, cylindrical and platelet particles. The radius (thickness) of active particles in the microstructure varies from 0.5 mm to 20 mm. Each simulation was operated with 2000 cycles. According to eqn (15)–(20), the SOC was influenced by the active material morphology and affected the SEI formation, exchange current density and the change of open circuit potential. The SEI thickness dSEI, exchange current density I0 and qU/qcs was recorded after the end of

Fig. 6 (a) The SEI thickness, (b) SOC, (c) qU/qcs and (d) exchange current density of spherical, cylinder and platelet particles during the first 2000 discharge–charge cycles. The radius of spherical particles is 2 mm. The radius of cylinder particles is 2 mm and the aspect ratio is 1 : 5. The thickness of cylinder particles is 4 mm and the aspect ratio is 1 : 10 : 10.

This journal is © the Owner Societies 2015

Phys. Chem. Chem. Phys., 2015, 17, 9812--9827 | 9819

View Article Online

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

PCCP

Fig. 7 Impedance response of a representative spherical, cylinder, and platelet active particle during the first 500 discharge–charge cycles. The radius of spherical particles is 2 mm. The radius of cylinder particles is 2 mm and the aspect ratio is 1 : 5. The thickness of cylinder particles is 4 mm and the aspect ratio is 1 : 10 : 10.

Paper

Fig. 8 Impedance response of porous electrode after 500, 1000 and 2000 cycles. The specific area, volume fraction and mean radius of the microstructure are 4000 cm1, 40% and 2.09 mm respectively.

Fig. 9 The porous electrode impedance response with diﬀerent specific surface area of active material. The volume fraction and mean particle radius of active material are 40% and 3 mm. (a) Particle-radius distribution with the specific area of 3500 cm1, 3000 cm1, 2500 cm1 and 2000 cm1. (b) The microstructure for (i) a = 3500 cm1 (without electrolyte), (ii) a = 3000 cm1, (iii) a = 2500 cm1, (iv) a = 2000 cm1. In the microstructure, the active material, binder, electrolyte and SEI layer are represented by the color of red, blue, purple and yellow respectively. (c) The porous electrode impedance response after 500 discharge–charge cycles. (d) The SEI resistance and charge transfer resistance after 500, 1000 and 2000 cycles.

9820 | Phys. Chem. Chem. Phys., 2015, 17, 9812--9827

This journal is © the Owner Societies 2015

View Article Online

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

Paper

charge process of each cycle. The results are represented in the following. The SEI thickness growth with cycling number is shown in Fig. 6(a). The spherical particles have the fastest side reaction rate, compared to the cylindrical and platelet particles. The reason is the same as the size eﬀect on SEI thickness. The SOC of spherical particle increases faster than cylindrical and platelet particles, according to eqn (15)–(17), which causes higher side reaction rate and thicker SEI thickness. The exchange current qU/qcs and I0 of different particle morphologies during cycling are shown in Fig. 6(c) and (d). Similar to the result of the size effect of spherical particles, the slope qU/qcs and exchange current density I0 are dominated by the SOC. Due to the variation of SOC, the platelet particles have the smallest value of qU/qcs and the spherical has the largest qU/qcs. Additionally, the exchange current density of spherical particles increases with the number of cycles (SOC 4 0.5), but the exchange current density of cylinder and platelet particles decrease with the number of cycles (SOC o 0.5) as shown in Fig. 6(d). Fig. 7 shows the impedance response varies with the particle morphologies after 500 cycles. The spherical particle has the largest SEI resistance while the platelet particle has the smallest

PCCP

SEI resistance, which is determined by the SEI thickness. The platelet particle has the largest charge transfer resistance while the cylindrical particle has the smallest charge transfer resistance due to the diﬀerence in exchange current I0. The morphology eﬀect on the diﬀusion resistance is attributed to the anisotropic of ion diﬀusion and the value of qU/qcs. The anisotropic of large curvature particle (e.g. platelet particles) increases the solid-phase diﬀusion resistance inside the particle. Eﬀect of electrode microstructure on impedance response In anodes, the particle-size distributions are diﬀerent according to electrode microstructures. The particle-size distribution determined three design aspects of porous electrode, which are (1) the specific surface area (cm1), (2) the volume fraction of active material and (3) the mean particle radius of the active material. As demonstrated above, the SEI thin layer, charge transfer resistance and diﬀusion resistance vary with the active particle size and morphology, which suggest strong dependence of the electrode microstructural variations (e.g. particle size distribution) on the impedance response. The impedance response of diﬀerent porous electrodes after cycling is as shown

Fig. 10 The porous electrode impedance response with diﬀerent volume fraction of active material. The specific area and mean particle radius of active material are 3000 cm1 and 3 mm. (a) Particle-radius distribution with 50%, 45%, 40% and 35% volume fraction of active material. (b) The microstructure for (i) 50% (without electrolyte), (ii) 45% (iii) 40% and (iv) 35% of active material. In the microstructure, the active material, binder and electrolyte are represented by the color of red, blue and purple respectively. (c) The porous electrode impedance response after 500 discharge–charge cycles. (d) The SEI resistance and charge transfer resistance after 500, 1000 and 2000 cycles.

This journal is © the Owner Societies 2015

Phys. Chem. Chem. Phys., 2015, 17, 9812--9827 | 9821

View Article Online

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

PCCP

in Fig. 8. As expected, due to the increase of SEI thickness, the SEI resistance increases during cycling. Influence of specific surface area. In order to keep the porosity and mean particle radius as a constant, the microstructure with larger surface area has a larger number of particles and smaller standard deviation as shown in Fig. 9(a) and (b). From Fig. 9(c) and (d), the impedance response shows that the microstructure with larger surface area has smaller resistance (SEI resistance, charge transfer resistance and solidphase diﬀusion resistance) in the electrode. The result can be explained from eqn (9)–(11) that the average admittance aYs increase with the surface area in the microstructure. Fig. 9(d) presents the increase of SEI resistance and charge transfer resistance during cycling. From the results, we can refer that the SEI thickness increases faster in the microstructure with small surface area. It is worth noticing that although the capacity lost increase with the (Brunauer–Emmett–Teller) BET surface area (m2 g1),26 increasing the surface area has a positive effect on the resistance. Influence of active material volume fraction. Fig. 10 shows the impedance response of the microstructures with diﬀerent

Paper

volume fraction of active material. According to the plot of particle-size distribution and the microstructure (Fig. 10(a) and (b)), it is found that the microstructure with smaller volume fraction of active material has more number of particles and smaller standard deviation. The electrode with a smaller volume fraction of active material has larger SEI resistance, but smaller charge transfer resistance and solid-phase diﬀusion resistance, as shown in Fig. 10(c) and (d). The larger SEI resistance means larger capacity lost, which agrees well with the previous results that the microstructure with larger BET specific area has larger capacity lost.26 The diﬀerence of the charge transfer resistance is attributed to that the average exchange current density I0 is smaller in the electrode with a smaller volume fraction of active material. The smaller solidphase diﬀusion resistance in the microstructure with smaller volume fraction of active material is mainly due to the lower average value of slope qU/qcs. Fig. 10(d) shows the increase of SEI resistance and charge transfer resistance. Diﬀerent from the influence of specific surface area, the influence of the volume fraction of active material to the SEI thickness increasing rate is not obvious.

Fig. 11 The porous electrode impedance response with varying mean particle radius. The specific area and volume fraction of active material are 4000 cm1 and 40%. (a) Particle-radius distribution of diﬀerent mean particle radius. (b) The microstructure for (i) Rmean = 2.8824 (without electrolyte) (ii) Rmean = 2.093 (iii) Rmean = 1.1035. In the microstructure, the active material, binder and electrolyte are represented by the color of red, blue and purple respectively. (c) The porous electrode impedance response after 500 discharge–charge cycles. (d) The SEI resistance and charge transfer resistance after 500, 1000 and 2000 cycles.

9822 | Phys. Chem. Chem. Phys., 2015, 17, 9812--9827

This journal is © the Owner Societies 2015

View Article Online

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

Paper

Influence of mean particle size. In the following, we investigated the influence of mean particle radius of the particle-size distribution on the electrodes. In our study, we varied the sharpness j in eqn (12) to change mean particle radius. The porous electrodes with specific areas of 4000 cm1 and 2000 cm1, and the sharpness of 1.0, 0.6 and 0.2 are discussed in this subsection. Fig. 11 and 12 show the eﬀects of mean particle radius Rmean on the porous electrode impedance response with specific areas of 4000 cm1 and 2000 cm1. From the particle-size distributions (Fig. 11(a) and 12(a)) and the microstructures (Fig. 11(b) and 12(b)), it can be found that the particle-size distributions in the electrode with 4000 cm1 specific area have a larger standard deviation than that in the electrode with 2000 cm1 specific area. In addition, in order to maintain the surface area while changing the mean particle radius, the range of Rmean we can change for a = 4000 cm1 is smaller than a = 2000 cm1. As shown in Fig. 11(c) and (d), the SEI resistance and solid-phase diﬀusion resistance decrease with Rmean but the charge transfer resistance increase with the decrease of Rmean in the electrode with 4000 cm1 specific surface area. On the opposite, the SEI resistance and charge

PCCP

transfer resistance increase with the decreasing of Rmean but the solid-phase diﬀusion resistance decreases with the Rmean in the electrode with 2000 cm1 specific surface area (Fig. 12(c) and (d)). The diﬀerence of SEI resistance with Rmean for the specific area of 4000 cm1 and 2000 cm1 is attributed to the particlesize distribution. For the particle-size distributions in Fig. 11(a) (a = 4000 cm1), the particles with radius smaller than 1 mm (SEI thickness decrease with the decrease of radius) has more influence on the SEI resistance when we averaged the impedance of active materials. On the contrary, for the particle-size distributions in Fig. 12(a) (a = 2000 cm1), since most of the particles radius are larger than 1 mm (the range SEI thickness increase with the decrease of radius), the SEI resistance decreases with the increase of Rmean. Therefore, for the electrodes with large specific surface area, the electrode should choose smaller particles (smaller Rmean) for smaller SEI resistance. As shown in Fig. 11(c) and 12(c), the charge transfer resistance increased with the decrease of Rmean for both specific surface areas of 2000 cm1 and 4000 cm1. It means that the distribution with small Rmean has smaller average exchange

Fig. 12 The porous electrode impedance response with varying mean particle radius. The specific area and volume fraction of active material are 2000 cm1 and 40%. (a) Particle-radius distribution of diﬀerent mean particle radius. (b) The microstructure for (i) Rmean = 5.7647 (without electrolyte) (ii) Rmean = 4.1852 (iii) Rmean = 2.2015. In the microstructure, the active material, binder and electrolyte are represented by the color of red, blue and purple respectively. (c) The porous electrode impedance response after 500 discharge–charge cycles. (d) The SEI resistance and charge transfer resistance after 500, 1000 and 2000 cycles.

This journal is © the Owner Societies 2015

Phys. Chem. Chem. Phys., 2015, 17, 9812--9827 | 9823

View Article Online

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

PCCP

Paper

Fig. 13 The porous electrode impedance response with spherical, cylinder and platelet particles. The specific area and volume fraction of the active material of electrode is 2000 cm1 and 40%. The aspect ratio of cylinder particles is 1 : 5. The aspect ratio of platelet particles is 1 : 10 : 10. (a) Particleradius distribution for spherical, cylinder and platelet particles (the morphology is as shown in Fig. 1). (b) The microstructure for (i) spherical (ii) cylinder (without electrolyte) (iii) platelet particles. In the microstructure, the active material, binder and electrolyte are represented by the color of red, blue and purple respectively. (c) The porous electrode impedance response after 500 discharge–charge cycles. (d) The SEI resistance and charge transfer resistance after 500, 1000 and 2000 cycles.

Fig. 14 (a) The specific surface area vs. the volume fraction of binder for the electrode with 2 mm spherical particles. (b) The SEI thickness with diﬀerent volume fraction of binder during the first 2000 discharge–charge cycles for the electrode with 2 mm spherical particles.

current density I0 than the one with large Rmean. The solid-phase diﬀusion resistance also depends on the Rmean of the distribution for both electrode microstructures. The solid-phase diﬀusion

9824 | Phys. Chem. Chem. Phys., 2015, 17, 9812--9827

resistance increased with Rmean in both cases because the particle-size distributions with large Rmean have longer diﬀusion distance and smaller qU/qcs than the ones with small Rmean.

This journal is © the Owner Societies 2015

View Article Online

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

Paper

PCCP

Fig. 15 (a) The porous electrode impedance response with diﬀerent volume fraction of binder for spherical particles. The specific area, volume fraction and radius of active material are 4500 cm1, 30% and 2 mm respectively. (b) The charge transfer resistance and SEI resistance after 500, 1000 and 2000 discharge–charge cycles.

The long diﬀusion distance and small qU/qcs for larger particles caused large diﬀusion resistance. In addition, Fig. 11(d) and 12(d) also show that the SEI resistance increasing speed is not changing with Rmean. Eﬀect of active particle morphology. The porous electrode impedance response with diﬀerent morphology of active material is shown in Fig. 13. According to the particle-size distributions and microstructures (see, Fig. 13(a) and (b)), it is found that spherical particles have more number of particles than the cylinder and platelet particles when the specific area is maintained at constant. As shown in Fig. 13(c) and (d), spherical particles have the largest SEI resistance and charge transfer resistance, while these particles have the smallest diﬀusion resistance. On the opposite, platelet particles have the smallest SEI resistance and charge transfer resistance, but the largest diﬀusion resistance. The electrode with spherical active material has the largest SEI resistance because the spherical particles has a thicker SEI thickness compared to the cylinder and platelet particles as shown in Fig. 6(a). The result of charge transfer resistance shows that under the same charging time and process, the electrode with the platelet active material has the largest exchange current density. For the solid-phase diﬀusion resistance, because spherical particles have shorter diﬀusion distance than the cylinder and platelet particles due to the curvature of particle surface, the electrodes with spherical particles have the smallest diﬀusion resistance. In addition, the largest qU/qcs of spherical particles is also a reason why spherical particles have the smallest diﬀusion resistance. In addition, from Fig. 13(d), the SEI resistance increasing rate is faster for spherical particles than the cylinder and platelet particles. Eﬀect of binder volume fraction. According to eqn (9)–(11), we know that the impedance strongly depends on the specific surface area (cm1). In realistic electrodes, the volume fraction of binder influences the interface surface area between the electrolyte and active material as shown in Fig. 14(a). Due to the decrease of surface area, under the same applied current, the current density (A cm2) will increase and affect the SEI

This journal is © the Owner Societies 2015

formation as shown in Fig. 14(b). Fig. 14(b) shows that the SEI thickness grows faster in the electrode with smaller volume fraction of binder. The SEI thickness decreases as binder increases because the increase of current density (A cm2) decreases the charging time (i.e. the surface concentration reaches the maximum value faster). However, although the SEI grew faster for a low volume fraction of binder, the electrode with 5% of binder has the smallest SEI resistance as shown in Fig. 15(a) and (b). It means the SEI resistance is dominated by the effective surface area between active material and electrolyte. Besides the SEI resistance, the charge transfer resistance and diffusion resistance also increase with the volume fraction of binder due to the diminishing of effective surface area. In addition, the SEI resistance increased faster for the electrode with 20% of the binder, as shown in Fig. 15(b), because the small effective surface area makes the SEI resistance grew faster than the one with the larger effective surface area.

Conclusions In this paper, the influence of electrode microstructural variability on the SEI formation and corresponding impedance response has been elucidated. In this regard, a microstructure-aware computational model has been presented which consists of physicochemical interactions pertinent to SEI formation in a typical LIB anode and elicits the influence thereof on the impedance characteristics. The impact of active particle morphology, size distribution, binder and electrolyte volume fractions on the SEI thickness, SOC, and the underlying interdependences of transport and interfacial resistances have been investigated in detail. This model enables a virtual diagnosis and characterization of the canonical mode of chemical degradation via prediction of the impedance spectra snapshots for intercalation electrodes. Due to the variation of particle-size distribution, the impedance response changes with active interfacial area, porosity, and mean particle size. The predictions suggest that the surface

Phys. Chem. Chem. Phys., 2015, 17, 9812--9827 | 9825

View Article Online

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

PCCP

area change dominates the impedance response. Moreover, the trade-oﬀ between the SEI resistance and charge transfer resistance has been found to be of critically dependent on the variation of the mean size of active particles and electrolyte volume fraction. From morphological variability, the spherical active particles show the largest SEI and charge transfer resistances compared to the cylindrical and platelet active particles. However, the spherical particles exhibit the lowest solid-phase diﬀusion resistance. The volume fraction of binder has been found to aﬀect the impedance response significantly. An increase of binder fraction decreases the interfacial active area, which in turn aﬀects the reaction current density, charging time and the SEI growth rate and hence ultimately on the impedance response. An important future development of this impedance model will include the eﬀect of phase transformation material, such as in LiFePO4, and concomitant dependence of solid-phase transport on crystallographic orientation. This will allow versatility of this microstructure-aware impedance model for a wide range of chemistry and materials choice.

Acknowledgements Financial support from NSF award no. 1438431 is gratefully acknowledged. The authors would like to thank Dr. Andreas Wiegmann from Math2Market GmbH for his support with electrode microstructure generation using GeoDict.

References 1 R. Wagner, N. Preschitschek, S. Passerini, J. Leker and M. Winter, J. Appl. Electrochem., 2013, 43, 481–496. 2 M. S. Whittingham, Chem. Rev., 2004, 104, 4271–4302. 3 B. L. Ellis, K. T. Lee and L. F. Nazar, Chem. Mater., 2010, 22, 691–714. 4 J. M. Tarascon and M. Armand, Nature, 2001, 414, 359–367. 5 F. Hao and D. Fang, J. Electrochem. Soc., 2013, 160, A595–A600. 6 S. Kalnaus, K. Rhodes and C. Daniel, J. Power Sources, 2011, 196, 8116–8124. 7 M. D. Levi and D. Aurbach, J. Electroanal. Chem., 1997, 421, 79–88. 8 M. D. Levi, E. A. Levi and D. Aurbach, J. Electroanal. Chem., 1997, 421, 89–97. 9 D. Aurbach, in Advances in Lithium-Ion Batteries, ed. W. A. van Schalkwijk and B. Scrosati, Academic/Plenem Publishers, New York, 2002, p. 7. 10 J. W. Jiang and J. R. Dahn, Electrochim. Acta, 2004, 49, 4599–4604. 11 C.-F. Chen, P. Barai and P. P. Mukherjee, J. Electrochem. Soc., 2014, 161, A2138–A2152. 12 P. Barai and P. P. Mukherjee, J. Electrochem. Soc., 2013, 160, A955–A967.

9826 | Phys. Chem. Chem. Phys., 2015, 17, 9812--9827

Paper

13 E. Prada, D. Di Domenico, Y. Creﬀ, J. Bernard, V. SauvantMoynot and F. Huet, J. Electrochem. Soc., 2013, 160, A616–A628. 14 E. Peled, J. Electrochem. Soc., 1979, 126, 2047–2051. 15 D. Aurbach, B. Markovsky, A. Shechter, Y. Ein-Eli and H. Cohen, J. Electrochem. Soc., 1996, 143, 3809–3820. 16 J. O. Besenhard, M. Winter, J. Yang and W. Biberacher, J. Power Sources, 1995, 54, 228–231. 17 K. Zaghib, G. Nadeau and K. Kinoshita, J. Electrochem. Soc., 2000, 147, 2110–2115. 18 S. Q. Shi, P. Lu, Z. Y. Liu, Y. Qi, L. G. Hector, H. Li and S. J. Harris, J. Am. Chem. Soc., 2012, 134, 15476–15487. 19 R. Fong, U. Vonsacken and J. R. Dahn, J. Electrochem. Soc., 1990, 137, 2009–2013. 20 R. Kanno, Y. Kawamoto, Y. Takeda, S. Ohashi, N. Imanishi and O. Yamamoto, J. Electrochem. Soc., 1992, 139, 3397–3404. 21 C. Lenain, L. Aymard, F. Salver-Disma, J. B. Leriche, Y. Chabre and J. M. Tarascon, Solid State Ionics, 1997, 104, 237–248. 22 P. Lu, C. Li, E. W. Schneider and S. J. Harris, J. Phys. Chem. C, 2014, 118, 896–903. 23 T. Zheng, A. S. Gozdz and G. G. Amatucci, J. Electrochem. Soc., 1999, 146, 4014–4018. 24 S. K. Rahimian, S. C. Rayman and R. E. White, J. Electrochem. Soc., 2010, 157, A1302–A1308. ´k, Electrochim. Acta, 2010, 55, 25 P. Verma, P. Maire and P. Nova 6332–6341. ´k and A. Monnier, J. Electrochem. Soc., 26 M. Winter, P. Nova 1998, 145, 428–436. 27 E. Barsoukov, S. H. Ryu and H. Lee, J. Electroanal. Chem., 2002, 536, 109–122. 28 J. P. Meyers, M. Doyle, R. M. Darling and J. Newman, J. Electrochem. Soc., 2000, 147, 2930–2940. 29 W. Gao, N. Singh, L. Song, Z. Liu, A. L. M. Reddy, L. Ci, R. Vajtai, Q. Zhang, B. Wei and P. M. Ajayan, Nat. Nanotechnol., 2011, 6, 496–500. 30 A. Zaban and D. Aurbach, J. Power Sources, 1995, 54, 289–295. 31 J. Fan and P. S. Fedkiw, J. Electrochem. Soc., 1997, 144, 399–408. 32 R. Koksbang, I. I. Olsen, P. E. Tonder, N. Knudsen and D. Fauteux, J. Appl. Electrochem., 1991, 21, 301–307. 33 F. Capuano, F. Croce and B. Scrosati, J. Electrochem. Soc., 1991, 138, 1918–1922. 34 G. Pistoia, A. Antonini, R. Rosati and C. Bellitto, J. Electroanal. Chem., 1996, 410, 115–118. 35 A. Lewandowski, B. Kurc, I. Stepniak and A. SwiderskaMocek, Electrochim. Acta, 2011, 56, 5972–5978. 36 E. Barsoukov, J. H. Kim, D. H. Kim, K. S. Hwang, C. O. Yoon and H. Lee, J. New Mater. Electrochem. Syst., 2000, 3, 301–308. 37 M. Jun, K. Smith and P. Graf, J. Power Sources, 2015, 273, 1226–1236. 38 J. Song and M. Z. Bazant, J. Electrochem. Soc., 2013, 160, A15–A24.

This journal is © the Owner Societies 2015

View Article Online

Published on 10 March 2015. Downloaded by University of Alberta on 27/04/2015 06:07:40.

Paper

39 J. Song and M. Z. Bazant, Electrochim. Acta, 2014, 131, 214–227. 40 B. Tribollet and J. Newman, J. Electrochem. Soc., 1984, 131, 2780–2785. 41 B. Tribollet and J. Newman, J. Electrochem. Soc., 1983, 130, 822–824. 42 R. W. J. M. Huang, F. Chung and E. M. Kelder, J. Electrochem. Soc., 2006, 153, A1459–A1465. 43 J. S. Newman and C. W. Tobias, J. Electrochem. Soc., 1962, 109, 1183–1191. 44 A. M. Johnson and J. Newman, J. Electrochem. Soc., 1971, 118, 510–517. 45 J. Newman and W. Tiedemann, AIChE J., 1975, 21, 25–41.

This journal is © the Owner Societies 2015

PCCP

46 S. K. Rahimian, S. Rayman and R. E. White, J. Power Sources, 2011, 196, 10297–10304. 47 Q. Zhang, E. Uchaker, S. L. Candelaria and G. Cao, Chem. Soc. Rev., 2013, 42, 3127–3171. 48 M. Guo, G. Sikha and R. E. White, J. Electrochem. Soc., 2011, 158, A122–A132. 49 B. S. Haran, B. N. Popov and R. E. White, J. Power Sources, 1998, 75, 56–63. 50 G. Ning and B. N. Popov, J. Electrochem. Soc., 2004, 151, A1584–A1591. 51 K. C. Smith, P. P. Mukherjee and T. S. Fisher, Phys. Chem. Chem. Phys., 2012, 14, 7040–7050.

Phys. Chem. Chem. Phys., 2015, 17, 9812--9827 | 9827